Abstract
The thermal and magnetic properties of uranium dioxide, a prime nuclear fuel and thoroughly studied actinide material, remain a long standing puzzle, a result of strong coupling between magnetism and lattice vibrations. The magnetic state of this cubic material is characterized by a 3k noncollinear antiferromagnetic structure and multidomain JahnTeller distortions, likely related to its anisotropic thermal properties. Here we show that single crystals of uranium dioxide subjected to strong magnetic fields along threefold axes in the magnetic state exhibit the abrupt appearance of positive linear magnetostriction, leading to a trigonal distortion. Upon reversal of the field the linear term also reverses sign, a hallmark of piezomagnetism. A switching phenomenon occurs at ±18 T, which persists during subsequent field reversals, demonstrating a robust magnetoelastic memory that makes uranium dioxide the hardest piezomagnet known. A model including a strong magnetic anisotropy, elastic, Zeeman, Heisenberg exchange, and magnetoelastic contributions to the total energy is proposed.
Introduction
Experimental studies carried out on UO_{2} under the cloak of the Manhattan Project showed the first hints of what later came to be accepted as antiferromagnetism (AFM) at T _{N} = 30.8 K^{1, 2}. Extensive neutronscattering measurements revealed noncollinear spin ordering with a 3k structure below T _{N} ^{3,4,5}. This is accompanied by a static JahnTeller distortion of the oxygen cage, and strong magnetoelastic interactions^{6,7,8,9} that emerge from a facecentered cubic (fcc) structure (see Fig. 1a, b). It was argued that a large thirdorder invariant in the free energy expansion that couples magnetic dipoles and electric quadrupoles^{6, 10, 11} results in the firstorder nature of this magnetoelastic transition. A dynamic JahnTeller model was also proposed^{12} to explain the persistence of strong magnetoelastic coupling well above T _{N}. Owing to the symmetry of the noncollinear 3k antiferromagnetic (AFM) order in UO_{2}, the existence of piezomagnetism (PZM) is possible^{13} but has never been observed. PZM, first predicted by Dzyaloshinsky^{14, 15}, is characterized by a linear coupling between the system’s mechanical strain and magnetic polarization. In PZM crystals, a magnetic moment can be induced by application of a physical stress, and it has captured attention in recent years as a mechanism that could be used in combination with multiferroics and piezoelectrics at the nanoscale to achieve control of magnetism by electric fields^{16}. Among the 122 space groups that describe magnetic order, only a subset of 66 can present PZM. It is precluded in the remaining 56 because they contain time reversal as a symmetry element (32 groups), its product with inversion (21 groups), or have spatialonly symmetries incompatible with the axial character of the PZM tensor (3 groups).
Here we have uncovered a magnetostriction (MS) linear in field, the converse of PZM^{17}, that confirms the noncollinear 3k nature of the magnetically ordered state in UO_{2}. High coercive fields of 18 T were found when the direction of applied magnetic field is reversed, making it the hardest piezomagnet known^{14, 16, 18,19,20,21}. These, together with previously unseen fieldinduced broken cubic symmetry and memory effects in UO_{2}, are likely related to complex magnetoelastic properties important for both applied and fundamental aspects. We propose a model Hamiltonian that is capable of reproducing the main experimental features.
Results
Axial and transverse MS
The MS, ε = ΔL/L (ppm), where ΔL is the sample length change with respect to the original length L, of UO_{2} was measured with applied magnetic fields up to 92.5 T along the [111] crystallographic direction, at various temperatures. In the paramagnetic (PM) state (T ≥ T _{N}) the axial MS ε _{a}(H), displayed in Fig. 1c, is negative and proportional to the square of the magnetic field. Upon cooling into the AFM state (T < T _{N}) in zero field, however, an additional positive linear term abruptly appears in the MS above a critical applied field. The MS can then be described by the expression ε _{a}(H, T) = α _{a}(T)H + β _{a} H ^{2}, with α _{a}(T) ≥ 0 and β _{a} < 0 for positive fields. The temperature dependence of the linear term α _{a}(T), Fig. 1c inset, shows characteristics of an order parameter. The quadratic term β _{a} is essentially constant in the entire experimental temperature range and is likely a consequence of the Zeeman effect on the U atom’s Γ_{5} triplet ground state, whose degeneracy is split into three singlets by the presence of a molecular field in the 3k state. Above T _{N} the results by Caciuffo et al.^{22} show that, even in the PM state, the triplet is split into three singlets, suggesting uncorrelated 1k dynamic JahnTeller distortions. A peculiar irreversible anomaly in the MS was observed when cooling the sample down in zero field (ZFC) and then sweeping the field past 18 T (see arrow). This behavior is described in more detail below. Additional MS data, taken in transverse geometry in a superconducting magnet to 15 T, Fig. 1d, show similar functional form ε _{t}(H, T) = α _{t}(T)H + β _{t} H ^{2} with α _{t}(T) ≤ 0 and β _{t} > 0. Taken together, ε _{a}(H, T) and ε _{t}(H, T) indicate a strong fieldinduced trigonal distortion of the zero field cubic lattice structure that changes sign upon entering the AFM state. When the axial and transverse strain at a constant field ε _{a,t}(H = 15 T, T) is considered, we notice in Fig. 1e that the onset of linear MS carries also a change in the Poisson ratio (ν = −ε _{t}/ε _{a}) from 0.4 in the PM state to 0.23 below T _{N}.
The ZFC axial MS measured at T = 2.5 K is shown again in Fig. 2a, alongside additional field sweeps identified with numbers. We see in trace 1 (dark blue) a very small ε _{a}(H) signal to H ≈ 10 T on the field upsweep, but then increases with increasing field, going through a local maximum at H ≤ 20 T. During the field downsweep the strain follows a monotonic linear decrease to zero with no visible remanence. Trace 2 (light grey) was measured in a subsequent negative magnetic field pulse, and ε _{a} was observed to turn negative, displaying a minimum and a rapid switch to positive values at approximately −18 T. Again, a monotonic decrease to zero strain with no remanence is observed during the field downsweep. Trace 3 (red) was measured during a second negative pulsed field, and a clear α _{a} H + β _{a} H ^{2} with α _{a}, β _{a} < 0 behavior is observed. That is, the same dependence on magnetic field shown in Fig. 1c (T = 2.2 K) but with a negative linear term is observed. When the field direction is changed once again, trace 4 (dark cyan) is obtained, displaying a minimum at 18 T and a rapid switch to positive values, with a monotonic decrease to zero as H is swept back to zero. Finally, when a second consecutive positive field is pulsed, trace 5 (orange), the strain is again a quadratic function of the magnetic field with α _{a} > 0 and β _{a} < 0.
We do not see any measurable remanence in the sample length on removal of the external field. There is, however, remanence in the response rate of the lattice, i.e., ∂ε/∂H. Figure 2b shows ∂ε _{a}/∂H = α _{a} + 2β _{a} H vs. H, computed from data in Fig. 2a. The area enclosed represents work performed by the magnetic field. Similar results (save opposite signs) were found for the strain measured perpendicular to the applied magnetic field, ∂ε _{t}/∂H = α _{t} + 2β _{t} H, in a superconducting magnet, and displayed in Fig. 2c, d. The fieldindependent terms α _{a} and α _{t} are related to the components of the magnetoelastic tensor Λ, as shown in the Supplementary Note 1. The expected theoretical ratio is α _{a}/α _{t} = −2 to be compared with the experimental ratio of 10.5/(−2.98) ≈ −3.52 (upper branch in Fig. 2b, lower branch in Fig. 2d). By symmetry considerations, the tensor Λ for UO_{2} has only three identical nonzero components (Λ _{14}) whose magnitude is 10^{−9 }Oe^{−1}, comparable to some of the highest known^{14, 18,19,20}. Λ _{14}, and consequently the α’s, are odd under time reversal, strongly suggesting that the system switches between magnetic states related by time reversal. The memory effect in the switching dynamics was investigated further by applying magnetic field pulses smaller than that necessary to achieve the equilibrium state. Immediately after cooling the sample in zero field, we show in Fig. 2e how a partial jump in ε _{a}(H) is obtained when magnetic field pulses of increasing magnitude were applied. This sequence was repeated for negative field direction. The reversible curve 1 (red) was obtained with a 5 T pulse. Irreversible curves, 2 (green) through 6 (purple), were obtained with peak fields between 6 and 14 T. Finally, the reversible curve 7 (orange) obtained with a pulse up to 18 T shows the equilibrium state. It is important to note that the envelope defined by these data sets follows very closely curve (1) in Fig. 2a, with smaller coercive field. We noticed that the fastest field sweep results in a higher coercive field (see Supplementary Note 3).
The interaction between magnetic field and AFM order in PZM systems, considered before by Scott and Anderson^{23} in the context of magnetite^{18}, only allows linear coupling when timereversal symmetry is nontrivially broken. Indeed, while all magnets break time reversal symmetry, AFMs fall into two categories: those where a symmetry element of the lattice can restore the original state after the t → −t transformation, and those where no such symmetry element exists in the lattice. The 3k order in UO_{2} displayed in Fig. 1b (space group Pa\(\overline 3 \), point group m \(\overline 3 \)) belongs to the latter^{3, 24,25,26} and hence allows a linear term in the MS. It has been postulated that the uranium 5f ordered magnetic moment of 1.74 μ _{B} ^{27}, strongly reduced from the 3.2 μ _{B} value expected for the J = 4 multiplet, is an indicator of the importance of combined crystal electric field effects and the JahnTeller coupling in UO_{2} ^{28}. These effects substantiate the possibility of a strong coupling between external fields and the Uatom environment^{12, 29}, breaking the degeneracy between states connected by a timereversal transformation.
One of our most remarkable findings is that UO_{2} shows a nonzero α _{a}, such that reversing the direction of the applied field changes the linear trigonal distortion from extension to compression until the switching field is exceeded, at which point the trigonal extension is recovered. A similar strain hysteresis or ‘butterfly’ memory loop, with significantly smaller switching fields, occurs in DyFeO_{3} ^{20}, where the switching is achieved via a rotation of the AFM vector (defined as the sum of U moments on face centers minus the moment on U corner in the U unit cell) between two equilibrium states connected by time reversal. The dependence of the MS tensor on the sign of the AFM vector causes the sign change of α. We think the mechanism at play in UO_{2} is similar, with magnetocrystalline anisotropy creating an energy barrier between two equilibrium states with opposite AFM vector. Indeed, when UO_{2} is ZFCcooled below T _{N}, a static JahnTeller distortion of the oxygen cage takes place, corresponding to a trigonal distortion compatible with the 8c Wyckoff position of the cubic space group (205) Pa \(\overline 3 \) (Fig. 1a, b). The consequent magnetic anisotropy generated by the distortion stabilizes a 3k transverse order (T _{A} in the notation described by Santini^{6}). As there are four different possible JahnTeller distortions, each one along a different cube diagonal, there are a total of eight possible degenerate 3k magnetic orders. Four of them have one of the four U magnetic moments along the [111] direction, and the other four are their timereversed states. From a magnetic point of view, there are thus only two domains with opposite AFM vector. At zero magnetic field, the eight degenerate domains can in principle coexist. When a positive magnetic field is applied along the [111] direction, the subset of four 3k domains with positive AFM vector is energetically favored. A negative [111] magnetic field favors domains with negative AFM vector. The same argument is valid for the structure labeled T _{B} by Santini^{6}. Our data in Fig. 2e suggest that the ZFC selection/rotation of domains happens gradually as the magnetic field is increased towards ~18 T. Once this highfield state is established, the domains remain stable even after complete removal of the magnetic field as demonstrated by the history dependence in the MS. The traces obtained, when plotted together, make a magnetoelastic butterfly evident. The lack of remanence mentioned above is then not surprising, as all states share the same zerofield lattice parameter a. If domain boundary effects are neglected, a change in the number or distribution implies neither contraction nor expansion of the sample.
Magnetization vs. magnetic field
Besides MS we also measured the magnetization of a UO_{2} crystal with H parallel to [111] (see Fig. 3a). The magnetic moment induced at 60 T, 0.5–0.6 μ _{B} per U, is still far from the estimated saturation value of 1.7 μ _{B} per U^{27}. Figure 3b shows the magnetization measured in positive and negative magnetic fields. When the dominant linear contribution is subtracted, a more complex structure becomes apparent. Black lines in Fig. 3c depict the magnetization after subtraction of a linear term on the first field pulse in each direction, right after ZFCing the sample. Green lines illustrate the data obtained on a second pulse in the same direction. A hysteretic behavior as well as a shoulder in the data at H = 18 T are clearly seen, which coincides with H _{coer} seen in the MS. The net magnetization at the shoulder might be consequence of a broken crystal symmetry in response to external fields.
Theoretical model
To model and understand the observed properties in UO_{2} we consider a minimalistic classical Hamiltonian where the degrees of freedom are the orientation of the magnetic moments at the four U atoms (4a positions) in the Pa \(\overline 3 \) unit cell. They are described by their projections along the cartesian coordinates \({\hat{\bf S}_{\rm{i}}} = \left[ {{\rm{sin}}\,{\theta _{\rm{i}}}\,{\rm{cos}}\,{\phi _{\rm{i}}}\,\hat {\bf x} + {\rm{sin}}\,{\theta _{\rm{i}}}\,{\rm{sin}}\,{\phi _{\rm{i}}}\,\hat {\bf y} + {\rm{cos}}\,{\theta _{\rm{i}}}\,\hat {\bf z}} \right]\) (see also Supplementary Note 2). The Hamiltonian includes: a Zeeman term that takes into account the interaction with the external field:
a magnetic anisotropy term stabilized by the static JahnTeller distortion of the oxygen cage:
where \({\hat {\bf v}_{\rm{i}}}\) are the unit vectors along the local anisotropy directions (1,1,1), \(\left( {\bar 1,\bar 1,1} \right)\), \(\left( {\bar 1,1,\bar 1} \right),\) \(\left( {1,\bar 1,\bar 1} \right)\) for the four U atoms, such that their vector sum is zero; a Heisenberg interaction compatible with the symmetry operations of the magnetic group:
where \({S_{{\rm{ir}}}}\left( {{{\hat {\bf v}}_{\rm{i}}}} \right)\) (r = x, y, z) are the three components of the magnetic moments with the z component along \({\hat {\bf v}_{\rm{i}}}\) ^{10, 11}. Here the sum accounts for the interactions between the four magnetic moments in the simple cubic unit cell and the factor four for the interaction with their images due to the periodic boundary conditions, the elastic energy of the cubic crystal:
the magnetoelastic energy:
proportional to the staggered magnetization
which is at the root of the PZM (see Supplementary Notes 1 and 2). At zero magnetic field, the anisotropy and Heisenberg terms are the only contributions to the Hamiltonian. They are responsible of the stabilization for the 3k AFM order.
The parameters A, J, E, and c _{44} were obtained following the criteria described in the Methods section below. The result of minimizing the total energy at T = 0 in this model are shown in Fig. 4, where the energetic stabilization of the magnetic domains with opposite AFM vector for positive and negative fields applied along [111] can be seen in Fig. 4a. The dependence of the deformation with the magnetic field is obtained from the energetic model by computing the derivative of the total energy with respect to the shear components of the strain tensor, with the result
with similar expressions for the other strain components showing the linear dependence of the deformation with the magnetic field. For a magnetic field along the [111] direction, the linear term
changes sign with the staggered magnetization M _{st} (Eq. (6)). The magnetization and deformation vs. magnetic field are shown in Fig. 4b, c, respectively. The model successfully reproduces the physics observed quantitatively, with a reasonable agreement for the MS slope and magnetization values, although the curvature in M(H) is more pronounced than in the experiment. It is notable that a quadrupole–quadrupole term is not required in our computations. The switching fields, with only the Zeeman terms present, however, are not reproduced in the model. As is well known^{6}, an auxiliary quadrupolar order parameter is thought to drive the firstorder nature of the AFM transition in zero field. One possibility is that piezomagnetic strain enhances the quadrupolar interaction strength, and causes the system to transition through the quadrupolar phase^{9, 30} at a certain value of the trigonal compression. Since the switching field varies depending on history and field sweep rates, crystal defects and impurities could also play a role. These lines of research are, however, beyond the scope of the present discussion and will be explored separately.
Conclusions
We have completed the first lowtemperature MS study of UO_{2} in magnetic fields up to 92.5 T, and uncovered a linear dependence on H consistent with predictions^{13} based on the noncollinear 3k magnetic order that breaks timereversal symmetry in a nontrivial way. This lowsymmetry state is the cause of PZM in UO_{2}. The record high coercive field of 18 T makes it a piezomagnet of formidable hardness^{14, 16, 18,19,20,21}. We propose a model Hamiltonian that is capable of reproducing the main experimental features, and points to the importance of a competition between exchange interactions and magnetic anisotropy. The unusually low thermal conductivity of UO_{2} cripples its performance as a fuel in nuclear reactors^{31}. Here we uncover firstorder coupling between the magnetism in Uatoms and lattice degrees of freedom that could be the origin of scattering of phonons against spin fluctuations dressed with dynamic JahnTeller oxygen modes^{22} well above T _{N}. These effects should be explored further. PZM, the magnetic counterpart to piezoelectricity^{32}, is also a property currently being discussed as a strategy to control magnetism by electricity^{16, 21} at the nanoscale. Our results and modeling on UO_{2}, applicable to other piezomagnets, could have an impact on current efforts in this direction. Inelastic neutron scattering as well as Xray scattering experiments in high magnetic field are planned to further test the details of the fieldinduced broken symmetries revealed by the results presented here.
Methods
Experimental
Several singlecrystal samples of UO_{2} were Xrayoriented, and cut in the shape of mmlong bars, each along a different principal crystallographic axis ([100], [110], and [111]). Variations in the sample length L as a function of the temperature and/or magnetic field ΔL/L = [L(H, T) − L(H _{0}, T _{0})]/L(H _{0}, T _{0}) were measured using a fiber Bragg grating (FBG) technique^{33,34,35} consisting of recording spectral information of the light reflected by a 0.5 mm long Bragg grating inscribed in the core of a 125 μm telecomtype optical fiber. The FBG section of the fiber is glued to the sample to be studied, and changes in the grating spacing are driven by changes in the sample dimension L along the fiber when temperature or magnetic field is changed. We use here the definition ε = ΔL/L, in units of parts per million (ppm). Capacitor bankdriven pulsed magnets were used to produce magnetic field pulses to 60 T, and a 100 T repetitive pulse magnet energized by a motor generator and a capacitor bank was used up to 92.5 T^{34, 35}. Owing to sample space limitations in pulsed magnets, the transverse MS was measured in a superconducting magnet furbished with a ^{4}He flow cryostat.
Computational
We used the Broyden–Fletcher–Goldfarb–Shanno algorithm as implemented in the open source SciPy package (http://www.scipy.org) for the energy minimization at T = 0. The anisotropy A = 2 meV and exchange J = 0.8 meV values are found necessary to obtain the experimental critical temperature T _{N} = 30.8 K using a standard Metropolis Monte Carlo algorithm at H = 0. A magnetoelastic interaction E = 0.280 meV T^{−1} is used to match the experimental value ε _{a}(H = 20 T) = 210 ppm. Other parameters used are the experimental shear elastic constant c _{44} = 60 GPa, the experimental lattice parameter a = 5.47 Å, g = 2, and S _{0} = 1.
Data availability
All data generated in this study are available from the authors upon request.
References
 1.
Jones, W. M., Gordon, J. & Long, E. A. The heat capacities of uranium, uranium trioxide, and uranium dioxide from 15 K to 300 K. J. Chem. Phys. 20, 695–699 (1952).
 2.
Leask, M. J. M., Roberts, L. E. J., Walter, A. J. & Wolf, W. P. Lowtemperature magnetic properties of some Uranium oxides. J. Chem. Soc. 1963, 47884794 (1963).
 3.
Burlet, P. et al. Neutron diffraction on actinides. J. Less Common Met. 121, 121–139 (1986).
 4.
Blackburn, E. et al. Spherical neutron spin polarimetry of anisotropic magnetic fluctuations in UO_{2}. Phys. Rev. B 72, 184411 (2005).
 5.
Caciuffo, R. et al. Anisotropic magnetic fluctuations in 3k antiferromagnets. J. Magn. Magn. Mater. 310, 1698–1702 (2007).
 6.
Santini, P. et al. Multipolar interactions in felectron systems: The paradigm of actinide dioxides. Rev. Mod. Phys. 81, 807–863 (2009).
 7.
Dolling, G. & Cowley, R. A. Observation of magnonphonon interaction at short wavelengths. Phys. Rev. Lett. 16, 683–685 (1966).
 8.
Cowley, R. A. & Dolling, G. Magnetic excitations in uranium dioxide. Phys. Rev. 167, 464–477 (1968).
 9.
Giannozzi, P. & Erdös, P. Theoretical analysis of the 3k magnetic structure and distortion of uranium dioxide. J. Mag. Mag. Mater. 67, 75–87 (1987).
 10.
Caciuffo, R. et al. Multipolar, magnetic, and vibrational lattice dynamics in the lowtemperature phase of uranium dioxide. −477Phys. Rev. B 84, 104409 (2011).
 11.
Carretta, S. et al. Quadrupolar waves in uranium dioxide. Phys. Rev. Lett. 105, 167201 (2010).
 12.
Amoretti, G. et al. 5felectron states in uranium dioxide investigated using highresolution neutron spectroscopy. Phys. Rev. B 40, 1856–1870 (1989).
 13.
Bar’yakhtar, V. G., Vitebskii, I. M. & Yablonskii, D. A. Magnetoelastic effects in noncollinear antiferromagnets. Zh. Eksp. Teor. Fiz. 89, 189–202 (1985).
 14.
BorovikRomanov, A. S. Piezomagnetism in the antiferromagnetic fluorides of cobalt and manganese. Sov. Phys. JETP 11, 786–793 (1960).
 15.
Dzialoshinskii, I. E. The problem of piezomagnetism. Sov. Phys. JETP 6, 621–622 (1958).
 16.
He, Q. et al. Electrically controllable spontaneous magnetism in nanoscale mixed phase multiferroics. Nat. Commun. 2, 225 (2011).
 17.
BorovikRomanov, A. S. Piezomagnetism, linear magnetostriction and magnetooptic effect. Ferroelectrics 162, 153–159 (1993).
 18.
Anderson, J. C., Birss, R. R. & Scott, R. A. M. Linear magnetostriction in hematite. Proc. Int. Conf. Magn. 597–599 (1964).
 19.
Prokhorov, A. S. & Rudashevskii, E. G. Magnetoelastic interactions and the singledomain antiferromagnetic state in cobalt fluoride. Kratk. Soobshch. Fiz. 11, 3–6 (1975).
 20.
Zvezdin, A. K. et al. Linear magnetostriction and antiferromagnetic domain structure in dysprosium orthoferrite. Sov. Phys. JETP 61, 645–647 (1985).
 21.
Zemen, J., Gercsi, Z. & Sanderman K. G. Piezomagnetic effect as a counterpart of negative thermal expansion in magnetically frustrated Mnbased antiperovskite nitrides. Preprint at http://arxiv.org/abs/1512.03470 (2015).
 22.
Caciuffo, R. et al. Magnetic excitations and dynamical JahnTeller distortions in UO_{2}. Phys. Rev. B 59, 13892–13900 (1999).
 23.
Scott, R. A. M. & Anderson, J. C. Indirect observation of AFM domains by linear magnetostriction. J. Appl. Phys. 37, 234–237 (1966).
 24.
Tinkham, M. Group Theory and Quantum Mechanics (McGrawHill, USA, 1964).
 25.
Tavger, B. A. Symmetry of piezomagnetic crystals. Sov. Phys. Crystallogr 3, 341–343 (1958).
 26.
Briss, R. R. & Anderson, J. C. Linear magnetostriction in antiferromagnetics. Proc. Phys. Soc 81, 1139–1140 (1963).
 27.
Faber, J. Jr. & Lander, G. H. Neutron diffraction study of UO_{2}. Antiferromagnetic state. Phys. Rev. B 14, 1151–1164 (1976).
 28.
Ippolito, D., Martinelli, L. & Bevilacqua, G. Dynamical JahnTeller effect on UO_{2}. Phys. Rev. B 71, 064419 (2005).
 29.
Zhou, F. & Ozolins, V. Crystal field and magnetic structure of UO_{2}. Phys. Rev 83, 085106 (2011).
 30.
Chen, H. H. & Levy, P. M. Dipole and quadrupole phase transitions in spin1 models. Phys. Rev. B 7, 4267–4284 (1973).
 31.
Gofryk, K. et al. Anisotropic thermal conductivity in uranium dioxide. Nat. Commun. 5, 4551 (2014).
 32.
Gautschi, G. Piezoelectric Sensorcs: Force, Strain, Pressure, Acceleration and Acoustic Emission Sensors, Materials and Amplifiers (Springer, NY, 2002).
 33.
Daou, R. et al. High resolution magnetostriction measurements in pulsed magnetic fields using fiber Bragg gratings. Rev. Sci. Instrum 81, 033909 (2010).
 34.
Jaime, M. et al. Magnetostriction and magnetic texture to 100.75 Tesla in frustrated SrCu_{2}(BO_{3})_{2}. Proc. Natl Acad. Sci. USA 110, 12404–12407 (2012).
 35.
Radtke, G., Saul, A., Dabkowska, H. A., Salamon, M. & Jaime, M. Magnetic nanopanthograph in the SrCu_{2} (BO_{3})_{2} ShastrySutherland lattice. Proc. Natl Acad. Sci. USA 112, 1971–1976 (2015).
Acknowledgements
Work by K.G. was supported by the U.S. Department of Energy, Office of Basic Energy Sciences, Materials Sciences, and Engineering Division project “Actinide materials under extreme conditions”. The NHMFL Pulsed Field Facility is supported by the NSF, the U.S. D.O.E., and the State of Florida through NSF cooperative grant DMR212 1157490. Work by N.H. and M.J. was supported by the U.S. D.O.E. BES project “Science at 100 Tesla”. We deeply thank the NHMFL 100 T magnet operation team: Y. Coulter, D. Roybal, M. Gordon, J. Martin, and H. Teshima. We thank A. Shethker, C.D. Batista, and J.F. Scott for their interest in our results and insightful discussions. A.S. thanks fruitful discussions with Céline Varvene and Jaejun Yu. M.B.S. gratefully acknowledges his visiting scientist status at NHMFL.
Author information
Affiliations
Contributions
K.G. proposed the experimental studies. M.J. and K.G. designed the research. M.J, V.S.Z., N.H., and K.G. performed the experiments. T.D., J.C.L., C.S., D.A.A., and J.L.S. provided the UO_{2} single crystal samples. A.S., M.J., and M.S. discussed and developed the theoretical model. A.S. performed the calculations. All authors discussed and interpreted the results, and contributed to the preparation and writing of the manuscript.
Corresponding authors
Ethics declarations
Competing interests
The authors declare no competing financial interests.
Additional information
Publisher's note: Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Electronic supplementary material
Rights and permissions
Open Access This article is licensed under a Creative Commons Attribution 4.0 International License, which permits use, sharing, adaptation, distribution and reproduction in any medium or format, as long as you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in a credit line to the material. If material is not included in the article’s Creative Commons license and your intended use is not permitted by statutory regulation or exceeds the permitted use, you will need to obtain permission directly from the copyright holder. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/.
About this article
Received
Accepted
Published
DOI
Further reading

Parametrization of LSDA+U for noncollinear magnetic configurations: Multipolar magnetism in UO2
Physical Review Materials (2019)

NanMTh6F30: A Large Family of Quaternary Thorium Fluorides
Crystal Growth & Design (2019)

Magnetoelastic coupling in URu2Si2 : Probing multipolar correlations in the hidden order state
Physical Review B (2019)

Magnetoelastic coupling across the fieldinduced transition of uranium mononitride
Physical Review B (2019)

Phase stabilization by electronic entropy in plutonium
Nature Communications (2019)
Comments
By submitting a comment you agree to abide by our Terms and Community Guidelines. If you find something abusive or that does not comply with our terms or guidelines please flag it as inappropriate.